Two-stage evolution from phosphate to sulfate of new KTP-type family members as UV nonlinear optical materials through chemical cosubstitution-oriented design.
He, Fangfang; Ge, Yuwei; Zhao, Xiaoyu; He, Jing; Huang, Ling; Gao, Daojiang; Bi, Jian; Wang, Xin; Zou, Guohong; Dalton transactions (Cambridge, England : 2003) 49 (2020) 5276–5282; doi:10.1039/d0dt00846j

data_7703874
_publ_section_title
;
 Two-stage evolution from phosphate to sulfate of new KTP-type family
 members as UV nonlinear optical materials through chemical
 cosubstitution-oriented design.
;
_journal_issue                   16
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              5276
_journal_page_last               5282
_journal_paper_doi               10.1039/d0dt00846j
_journal_volume                  49
_journal_year                    2020
_chemical_formula_sum            'F H6 N O5 P Sb'
_chemical_formula_weight         271.78
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   difmap
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2019-04-01 deposited with the CCDC.	2020-03-26 downloaded from the CCDC.
;
_cell_angle_alpha                68.272(3)
_cell_angle_beta                 68.966(3)
_cell_angle_gamma                89.938(4)
_cell_formula_units_Z            2
_cell_length_a                   6.5374(4)
_cell_length_b                   6.5425(5)
_cell_length_c                   8.3743(6)
_cell_measurement_reflns_used    5865
_cell_measurement_temperature    150(2)
_cell_measurement_theta_max      56.629
_cell_measurement_theta_min      5.677
_cell_volume                     306.95(4)
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_temperature      150(2)
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Bruker D8'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0580
_diffrn_reflns_av_unetI/netI     0.0363
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.997
_diffrn_reflns_limit_h_max       8
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            9316
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.997
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         28.350
_diffrn_reflns_theta_min         2.838
_exptl_absorpt_coefficient_mu    4.735
_exptl_crystal_density_diffrn    2.941
_exptl_crystal_description       flakelike
_exptl_crystal_F_000             256
_refine_diff_density_max         3.215
_refine_diff_density_min         -1.805
_refine_diff_density_rms         0.258
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.973
_refine_ls_hydrogen_treatment    refall
_refine_ls_matrix_type           full
_refine_ls_number_parameters     106
_refine_ls_number_reflns         1541
_refine_ls_number_restraints     6
_refine_ls_restrained_S_all      0.972
_refine_ls_R_factor_all          0.0396
_refine_ls_R_factor_gt           0.0344
_refine_ls_shift/su_max          0.003
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0753P)^2^+0.6096P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0910
_refine_ls_wR_factor_ref         0.0948
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1400
_reflns_number_total             1541
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d0dt00846j2.cif
_cod_data_source_block           mo_0123_6_0ma
_cod_depositor_comments
'Adding full bibliography for 7703873--7703874.cif.'
_cod_database_code               7703874
_shelx_shelxl_version_number     2014/7
_shelx_res_checksum              37425